SUPERSEDED (click for Active standard)
| ||Format||Pages||Price|| |
|6||$54.00||  ADD TO CART|
1.1 This specification covers electric-fusion-welded steel pipe suitable for corrosive service.
Note 1—The dimensionless designator NPS (nominal pipe size) has been substituted in this specification for traditional terms such as nominal diameter, size, and nominal size.
1.2 This specification covers grades of ferritic/austenitic steel as indicated in Table 1. The selection of the proper alloy and requirements for heat treatment shall be at the discretion of the purchaser, dependent on the service conditions to be encountered.
1.3 Five classes of pipe are covered as follows:
1.3.1 Class 1—Pipe shall be double welded by processes using filler metal in all passes and shall be radiographed completely.
1.3.2 Class 2—Pipe shall be double welded by processes using filler metal in all passes. No radiograph is required.
1.3.3 Class 3—Pipe shall be single welded by processes using filler metal in all passes and shall be radiographed completely.
1.3.4 Class 4—Same as Class 3, except that the weld pass exposed to the inside pipe surface is permitted to be made without the addition of filler metal (see 22.214.171.124 and 126.96.36.199).
1.3.5 Class 5—Pipe shall be double welded by processes using filler metal in all passes and shall be spot radiographed.
1.4 Supplementary requirements covering provisions ranging from additional testing to formalized procedures for manufacturing practice are provided. Supplementary Requirements S1 through S4 are included as options to be specified in the purchase order when desired.
1.5 The values stated in either SI units or inch-pound units are to be regarded separately as standard. Within the text, the SI units are shown in brackets. The values stated in each system may not be exact equivalents; therefore, each system shall be used independently of the other. Combining values from the two systems may result in non-conformance with the standard. The inch-pound units shall apply unless the M designation of the specification is specified in the order.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
A240/A240M Specification for Chromium and Chromium-Nickel Stainless Steel Plate, Sheet, and Strip for Pressure Vessels and for General Applications
A480/A480M Specification for General Requirements for Flat-Rolled Stainless and Heat-Resisting Steel Plate, Sheet, and Strip
A941 Terminology Relating to Steel, Stainless Steel, Related Alloys, and Ferroalloys
A999/A999M Specification for General Requirements for Alloy and Stainless Steel Pipe
E426 Practice for Electromagnetic (Eddy-Current) Examination of Seamless and Welded Tubular Products, Titanium, Austenitic Stainless Steel and Similar Alloys
ASME Boiler and Pressure Vessel CodeSection III Section IX Section VIII
ICS Number Code 25.160.40 (Welding joints and welds)
UNSPSC Code 31311509(Stainless steel welded or brazed pipe assemblies)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM A928 / A928M-11, Standard Specification for Ferritic/Austenitic (Duplex) Stainless Steel Pipe Electric Fusion Welded with Addition of Filler Metal, ASTM International, West Conshohocken, PA, 2011, www.astm.orgBack to Top